Spreadsheet: 0f2dad1c-9047-481c-99f0-12cd97ea98de
Sheet: Sheet1

Material Name | EL | ET | ER | GLT | GLR | GTR | nLT | nLR | nTR | r | Fiber Ultimate Strength | Transverse Ultimate Strength | Fiber Ultimate Strength.1 | Transverse Ultimate Strength.1 | Ultimate Shear Strength | Unnamed: 16 | CTE | Unnamed: 18 | Unnamed: 19 | CTE.1 | CTE.2 | Loss Factor | Loss Factor.1 | Loss | Shrinkage | Shrinkage.1 | Source | Unnamed: 28
 | (Msi) | (Msi) | (Msi) | (Msi) | (Msi) | (Msi) |  |  |  | (lb/in3) | Tension | Tension | Compression | Compression | (Ksi) |  | (L) |  |  | (T) | (R) | (L) | (T) | Factor | (Radial) | (Tangential)
 |  |  |  |  |  |  |  |  |  |  | (Ksi) | (Ksi) | (Ksi) | (Ksi) |  |  | (10-6 in/in oF) |  |  | (10-6 in/in oF) | (10-6 in/in oF) |  |  | (R) | (%) | (%)
Balsa (5 lb/ft3), (softwood) | 0.22 | 0.0033 | 0.0102 | 0.0082 | 0.012 | 0.0011 | 0.009 | 0.018 | 0.231 | 0.0029 | 0 | 0 | 0.51 | 0 | 0.08 |  | 0 |  |  | 24.1 | 16.3 | 0 | 0 | 0 | - | - | U.S. Defense Dept, ANC-18 (1951)/Mil Handbook 23 (1968), (B-Basis Allowables)
Balsa (6 lb/ft3), (softwood) | 0.31 | 0.0047 | 0.0144 | 0.0116 | 0.0169 | 0.0016 | 0.009 | 0.018 | 0.231 | 0.0035 | 0 | 0 | 0.74 | 0 | 0.1 |  | 0 |  |  | 24.1 | 16.3 | 0 | 0 | 0 | - | - | U.S. Defense Dept, ANC-18 (1951)/Mil Handbook 23 (1968), (B-Basis Allowables)
Balsa (7 lb/ft3), (softwood) | 0.4 | 0.0061 | 0.0186 | 0.0149 | 0.0218 | 0.002 | 0.009 | 0.018 | 0.231 | 0.0041 | 0 | 0 | 0.86 | 0 | 0.12 |  | 0 |  |  | 24.1 | 16.3 | 0 | 0 | 0 | - | - | U.S. Defense Dept, ANC-18 (1951)/Mil Handbook 23 (1968), (B-Basis Allowables)
Balsa (8 lb/ft3), (softwood) | 0.5 | 0.0074 | 0.0228 | 0.0183 | 0.0267 | 0.0025 | 0.009 | 0.018 | 0.231 | 0.0046 | 0 | 0 | 1.18 | 0 | 0.14 |  | 0 |  |  | 24.1 | 16.3 | 0 | 0 | 0 | - | - | U.S. Defense Dept, ANC-18 (1951)/Mil Handbook 23 (1968), (B-Basis Allowables)
Balsa (9 lb/ft3), (softwood) | 0.59 | 0.0088 | 0.027 | 0.0217 | 0.0316 | 0.0029 | 0.009 | 0.018 | 0.231 | 0.0052 | 0 | 0 | 1.4 | 0 | 0.15 |  | 0 |  |  | 24.1 | 16.3 | 0 | 0 | 0 | - | - | U.S. Defense Dept, ANC-18 (1951)/Mil Handbook 23 (1968), (B-Basis Allowables)
Balsa (10 lb/ft3), (softwood) | 0.68 | 0.0102 | 0.0312 | 0.0251 | 0.0366 | 0.0034 | 0.009 | 0.018 | 0.231 | 0.0058 | 0 | 0 | 1.64 | 0 | 0.17 |  | 0 |  |  | 24.1 | 16.3 | 0 | 0 | 0 | - | - | U.S. Defense Dept, ANC-18 (1951)/Mil Handbook 23 (1968), (B-Basis Allowables)
Balsa (11 lb/ft3), (softwood) | 0.77 | 0.0115 | 0.0354 | 0.0285 | 0.0415 | 0.0038 | 0.009 | 0.018 | 0.231 | 0.0064 | 0 | 0 | 1.85 | 0 | 0.19 |  | 0 |  |  | 24.1 | 16.3 | 0 | 0 | 0 | - | - | U.S. Defense Dept, ANC-18 (1951)/Mil Handbook 23 (1968), (B-Basis Allowables)
Balsa (12 lb/ft3), (softwood) | 0.85 | 0.0128 | 0.0392 | 0.0315 | 0.046 | 0.0043 | 0.009 | 0.018 | 0.231 | 0.0069 | 0 | 0 | 2.07 | 0 | 0.21 |  | 0 |  |  | 24.1 | 16.3 | 0 | 0 | 0 | - | - | U.S. Defense Dept, ANC-18 (1951)/Mil Handbook 23 (1968), (B-Basis Allowables)
Balsa (15 lb/ft3), (softwood) | 1.12 | 0.0167 | 0.0513 | 0.0413 | 0.0602 | 0.0056 | 0.009 | 0.018 | 0.231 | 0.0087 | 0 | 0 | 2.74 | 0 | 0.27 |  | 0 |  |  | 24.1 | 16.3 | 0 | 0 | 0 | - | - | U.S. Defense Dept, ANC-18 (1951)/Mil Handbook 23 (1968), (B-Basis Allowables)
Baldcypress, (softwood) | 1.24 | 0Â=60 height=18> | 0Â | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0185 | 9.6 | 0.14 | 5.4 | 0.94 | 0.84 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 3.8 | 6.2 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
 |  | 1.24
Cedar, Alaska, (softwood) | 1.22 | 0Â | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0179 | 9.9 | 0.18 | 5.1 | 0.81 | 0.93 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 2.8 | 6 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Cedar, Northern white-, (softwood) | 0.69 | 0Â | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0127 | 6 | 0.12 | 3.3 | 0.43 | 0.7 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 2.1 | 4.7 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Cedar, Port Orford, (softwood) | 1.43 | 0Â | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0168 | 10.2 | 0.16 | 5.5 | 0.81 | 0.79 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 4.6 | 6.9 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Cedar, Western Redcedar, (softwood) | 0.96 | 0Â | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0133 | 7.1 | 0.11 | 4.2 | 0.64 | 0.72 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 2.4 | 5 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Fir, [NAME], (softwood) | 1.48 | 0.074 | 0.1006 | 0.1154 | 0.0947 | 0.0104 | 0.029 | 0.036 | 0.374 | 0.0191 | 10.9 | 0.14 | 5.6 | 1.02 | 0.93 |  | 3.16 |  |  | 42.7 | 27.9 | 0 | 0 | 0 | 5 | 7.8 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Fir, California Red, (softwood) | 1.32 | 0.066 | 0.0898 | 0.103 | 0.0845 | 0.0092 | 0.029 | 0.036 | 0.374 | 0.0162 | 9.4 | 0.19 | 4.7 | 0.68 | 0.89 |  | 3.16 |  |  | 42.7 | 27.9 | 0 | 0 | 0 | 4.5 | 7.9 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Fir, Noble, (softwood) | 1.47 | 0.0735 | 0.1 | 0.1147 | 0.0941 | 0.0103 | 0.029 | 0.036 | 0.374 | 0.0162 | 9.8 | 0.11 | 4.8 | 0.7 | 0.88 |  | 3.16 |  |  | 42.7 | 27.9 | 0 | 0 | 0 | 4.5 | 8.3 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Fir, Pacific, (softwood) | 1.32 | 0.066 | 0.0898 | 0.103 | 0.0845 | 0.0092 | 0.029 | 0.036 | 0.374 | 0.0156 | 8.4 | 0.13 | 4.5 | 0.53 | 0.83 |  | 3.16 |  |  | 42.7 | 27.9 | 0 | 0 | 0 | 4.5 | 10 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Fir, White, (softwood) | 1.17 | 0.0585 | 0.0796 | 0.0913 | 0.0749 | 0.0082 | 0.029 | 0.036 | 0.374 | 0.015 | 8.4 | 0.13 | 4.4 | 0.65 | 0.78 |  | 3.34 |  |  | 32.6 | 21.8 | 0 | 0 | 0 | 3.2 | 7 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Hemlock, Western, (softwood) | 1.51 | Â 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0174 | 11 | 0.15 | 5.5 | 0.73 | 0.86 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 4.3 | 7.9 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Incense-Cedar, California, (softwood) | 0.9 | Â 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0145 | 7.6 | 0.14 | 4.5 | 0.79 | 0.76 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 3.3 | 5.2 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Larch, Western, (softwood) | 1.48 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0214 | 11 | 0.14 | 6.4 | 1.15 | 1.11 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 4.2 | 8.1 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Pine, Eastern White, (softwood) | 1.06 | Â 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0145 | 7.6 | 0.15 | 4 | 0.52 | 0.74 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 2.1 | 6.1 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Pine, Ponderosa, (softwood) | 1.07 | Â 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0162 | 8.1 | 0.19 | 4.2 | 0.75 | 0.9 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 3.9 | 6.3 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Pine, Red, (softwood) | 1.53 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0191 | 10.8 | 0.19 | 5.8 | 0.82 | 0.97 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 4.6 | 7.2 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Pine, Sugar, (softwood) | 1.02 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.015 | 7.3 | 0.16 | 4 | 0.63 | 0.83 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 2.9 | 5.6 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Pine, Western White, (softwood) | 1.28 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0162 | 8.3 | 0.19 | 4.6 | 0.56 | 0.7 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 4.1 | 7.4 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Redwood, old-growth, (softwood) | 1.34 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0145 | 10 | 0.24 | 6.15 | 0.7 | 0.94 |  | 4.28 |  |  | 35.1 | 23.6 | 0 | 0 | 0 | - | - | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Redwood, Young-growth, (softwood) | 1.1 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0126 | 7.9 | 0.25 | 5.22 | 0.52 | 1.11 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | - | - | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Spruce, Red, (softwood) | 1.32 | 0.0568 | 0.103 | 0.0805 | 0.0845 | 0.004 | 0.02 | 0.03 | 0.278 | 0.0162 | 9.3 | 0.16 | 4.9 | 0.63 | 0.89 |  | 3.15 |  |  | 32.3 | 23.8 | 0.0111 | 0.0166 | 0.0166 | 3.8 | 7.8 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Spruce, [NAME], (softwood) | 1.38 | 0.0593 | 0.1076 | 0.0842 | 0.0883 | 0.0041 | 0.02 | 0.03 | 0.278 | 0.0162 | 9.4 | 0.17 | 4.7 | 0.74 | 0.99 |  | 3.15 |  |  | 32.3 | 23.8 | 0.0111 | 0.0166 | 0.0166 | 4.2 | 7.5 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Spruce, White, (softwood) | 1.15 | 0.0495 | 0.0897 | 0.0702 | 0.0736 | 0.0035 | 0.02 | 0.03 | 0.278 | 0.0168 | 8.7 | 0.16 | 4.4 | 0.59 | 0.85 |  | 3.15 |  |  | 32.3 | 23.8 | 0.0111 | 0.0166 | 0.0166 | 4.7 | 8.2 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Alder, (hardwood) | 1.38 | 0Â | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0148 | 9.8 | 0.39 | 5.82 | 0.44 | 1.08 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | - | - | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Ash, black, (hardwood) | 1.31 | 0.0838 | 0.1428 | 0.0537 | 0.0747 | 0.0216 | 0.0421 | 0.0582 | 0.386 | 0.0203 | 10.6 | 0.32 | 4.6 | 0.94 | 1.19 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 5 | 7.8 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Ash, commercial white, (hardwood) | 1.4 | 0.0896 | 0.1526 | 0.0574 | 0.0798 | 0.0231 | 0.0421 | 0.0582 | 0.386 | 0.0237 | 13.2 | 0.38 | 6.1 | 1.68 | 1.59 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 4.5 | 7.2 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Aspen, Bigtooth, (hardwood) | 1.43 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0141 | 9.1 | 0.26 | 5.3 | 0.45 | 1.08 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | - | - | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Aspen, Quaking, (hardwood) | 1.18 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0137 | 8.4 | 0.26 | 4.25 | 0.37 | 0.85 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | - | - | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Basswood, (hardwood) | 1.22 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0145 | 7.7 | 0.17 | 3.8 | 0.45 | 0.77 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 6.6 | 9.3 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Beech, (hardwood) | 1.48 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0249 | 13.2 | 0.46 | 6 | 1.3 | 1.59 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 5.1 | 11 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Birch, Alaska, (hardwood) | 1.58 | 0.079 | 0.1232 | 0.1074 | 0.1169 | 0.0269 | 0.024 | 0.043 | 0.426 | 0.022 | 11.8 | 0.46 | 5.8 | 0.85 | 1.12 |  | 3.36 |  |  | 38.3 | 30.7 | 0.0143 | 0.0407 | 0.0407 | 6.5 | 9.9 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Birch, Paper, (hardwood) | 1.34 | 0.067 | 0.1045 | 0.0911 | 0.0992 | 0.0228 | 0.024 | 0.043 | 0.426 | 0.022 | 10.6 | 0.24 | 4.5 | 0.74 | 0.98 |  | 3.36 |  |  | 38.3 | 30.7 | 0.0143 | 0.0407 | 0.0407 | 6.3 | 8.6 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Birch, [NAME], (hardwood) | 2.17 | 0.1085 | 0.1693 | 0.1476 | 0.1606 | 0.0369 | 0.024 | 0.043 | 0.426 | 0.0235 | 16.9 | 0.95 | 8.54 | 1.08 | 2.24 |  | 3.36 |  |  | 38.3 | 30.7 | 0.0143 | 0.0407 | 0.0407 | 6.8 | 8.8 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Birch, [NAME], (hardwood) | 2.01 | 0.1005 | 0.1568 | 0.1367 | 0.1487 | 0.0342 | 0.024 | 0.043 | 0.426 | 0.0224 | 16.6 | 0.92 | 8.17 | 0.97 | 1.88 |  | 3.36 |  |  | 38.3 | 30.7 | 0.0143 | 0.0407 | 0.0407 | 6.8 | 8.8 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
[NAME], Black, (hardwood) | 1.31 | Â 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0208 | 14.3 | 0.28 | 5.8 | 0.88 | 1.36 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 3.7 | 7.1 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Cottonwood, (hardwood) | 1.15 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0162 | 7.7 | 0.27 | 4 | 0.49 | 0.76 |  | 2.89 |  |  | 32.6 | 23.2 | 0 | 0 | 0 | 3.9 | 9.2 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Elm, American, (hardwood) | 1.16 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0203 | 10.6 | 0.32 | 4.6 | 0.88 | 1.2 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 4.2 | 9.5 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Elm, Rock, (hardwood) | 1.31 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0249 | 13.5 | 0.3 | 5.9 | 1.55 | 1.53 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 4.8 | 8.1 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Hickory, (hardwood) | 1.78 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0289 | 17.1 | 0.3 | 7.2 | 2.25 | 1.66 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 7.4 | 11.4 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Khaya, (hardwood) | 1.26 | 0.063 | 0.1399 | 0.0743 | 0.1109 | 0.0265 | 0.032 | 0.033 | 0.264 | 0.0185 | 9.8 | 0.23 | 5 | 1.32 | 1.11 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 4.1 | 5.8 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Locust, Black, (hardwood) | 1.81 | 0Â | 0 | 0 | 0 | 0 | 0 | 0 | Â 0 | 0.0284 | 18.1 | 0.34 | 9 | 2.45 | 2.01 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 4.4 | 6.9 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)
Magnolia, Southern, (hardwood) | 1.2 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | Â 0 | 0.0203 | 10.1 | 0.35 | 4.5 | 1.1 | 1.23 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 5.4 | 6.6 | Design of Wood Aircraft Structures, U.S. Defense Dept/Forest Products Lab, ANC-18 (Nominal Property)
Mahogany, (hardwood) | 1.37 | 0.0877 | 0.1466 | 0.0904 | 0.1178 | 0.0384 | 0.034 | 0.033 | 0.326 | 0.0203 | 14.7 | 0.17 | 6.2 | 1.37 | 1.06 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 3.5 | 4.8 | Design of Wood Aircraft Structures, U.S. Defense Dept/Forest Products Lab, ANC-18 (Nominal Property)
[NAME], (hardwood) | 0.99 | 0 | 0Â | 0Â | 0Â | 0Â | 0 | 0 | 0 | 0.0191 | 8.1 | 0.26 | 4.2 | 0.93 | 1.2 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 3 | 7.2 | Design of Wood Aircraft Structures, U.S. Defense Dept/Forest Products Lab, ANC-18 (Nominal Property)
Maple, Sugar, (hardwood) | 1.59 | 0 | 0Â | 0 | 0 | 0Â | 0Â | 0Â | 0Â | 0.0249 | 14.1 | 0.26 | 6.5 | 1.79 | 1.83 |  | 3.82 |  |  | 35.3 | 26.8 | 0.0001 | 0.0385 | 0.0385 | 4.9 | 9.5 | Design of Wood Aircraft Structures, U.S. Defense Dept/Forest Products Lab, ANC-18 (Nominal Property)
Oak, (hardwood) | 1.46 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0 | 0.0255 | 12.3 | 0.38 | 5.7 | 1.45 | 1.47 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 4.8 | 9.4 | Design of Wood Aircraft Structures, U.S. Defense Dept/Forest Products Lab, ANC-18 (Nominal Property)
Pecan, (hardwood) | 1.48 | Â 0 | Â 0 | Â 0 | Â 0 | Â 0 | Â 0 | 0Â | 0Â | 0.0266 | 12.8 | 0.4 | 6.5 | 2.12 | 1.69 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 4.9 | 8.9 | Design of Wood Aircraft Structures, U.S. Defense Dept/Forest Products Lab, ANC-18 (Nominal Property)
Poplar, [NAME], (hardwood) | 1.25 | 0.0538 | 0.115 | 0.0863 | 0.0938 | 0.0138 | 0.019 | 0.03 | 0.329 | 0.0168 | 8.6 | 0.25 | 4.1 | 0.62 | 0.93 |  | 3.17 |  |  | 29.7 | 27.8 | 0 | 0 | 0 | 4 | 7.1 | Design of Wood Aircraft Structures, U.S. Defense Dept/Forest Products Lab, ANC-18 (Nominal Property)
Sweetgum, (hardwood) | 1.34 | 0.067 | 0.1541 | 0.0817 | 0.1193 | 0.0281 | 0.023 | 0.044 | 0.309 | 0.0203 | 11.2 | 0.36 | 4.8 | 0.77 | 1.17 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 5.2 | 9.9 | Design of Wood Aircraft Structures, U.S. Defense Dept/Forest Products Lab, ANC-18 (Nominal Property)
Sycamore, (hardwood) | 1.2 | Â 0 | Â 0 | 0Â | Â 0 | 0Â | Â 0 | 0 | 0 | 0.0203 | 9.4 | 0.35 | 4.5 | 0.89 | 1.18 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 5.1 | 7.6 | Design of Wood Aircraft Structures, U.S. Defense Dept/Forest Products Lab, ANC-18 (Nominal Property)
Walnut, (hardwood) | 1.46 | 0.0818 | 0.1548 | 0.0905 | 0.1241 | 0.0305 | 0.036 | 0.052 | 0.367 | 0.022 | 13.3 | 0.33 | 6.4 | 1.27 | 1.18 |  | 0 |  |  | 0 | 0 | 0 | 0 | 0 | 5.2 | 7.1 | Design of Wood Aircraft Structures, U.S. Defense Dept, ANC-18, 1951. (Nominal Property)